Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites


 Clementine Phillips
 1 years ago
 Views:
Transcription
1 Aspect Ratio Requirements for NanotubeReinforced, PolymerMatrix Composites J.A.Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Abstract A fiber s efficiency in a shortfiber composite can be accurately solved by shearlag methods, which can account for fiber geometry, an imperfect interface (or interphase), and extend to low volume fractions. Such an analysis was used to evaluate the aspect ratio requirements for singlewalled nanotubes (SWNT) in a polymeric composite and contrast it to conventional fibers. The aspect ratio requirements are indistinguishable among all stiff fibers, except at low volume fractions where stiffer fibers require higher aspect ratios. The required aspect ratio decreases significantly at higher volume fractions. A scaling effect in the interphase term implies the interphase is more important for nanofibers than for larger fibers. If the interface between nanofibers and the matrix is not excellent, those fibers will not provide effective reinforcement. The most promising SWNT composites should use higher volume fractions and focus on systems where the fiber can stiffen the matrix in the interphase region. Key words: A. Fibres, B. Nanostructures, C. Interface/interphase, D. Analytical modelling. Introduction A common model for aligned shortfiber composite modulus, E c, simply modifies the standard rule of mixtures [, 2]. For nanotubes reinforcement, this model takes the form E c = η f E ( zz φv f + E m V m () where η f is a fiber efficiency factor, E zz ( is the nanotube wall axial modulus, E m is the matrix modulus, and V f and V m are the fiber and matrix volume fractions. The fiber volume fraction is taken as inclusive of the hollow space within the nanotubes (for better comparison with solid fiber results). The factor φ is the fraction of the nanotube occupied by wall material (i.e., the volume fraction of nanotube walls with modulus E zz ( is V w = φv. The fiber efficiency factor, η f, is a short fiber s load bearing capability relative to the analogous continuous fiber. It can be calculated from a concentric cylinders model (CCM) for a fiber of length l embedded in a matrix cylinder. The fiber has zero load on the ends while the matrix carries the entire applied load (see Fig. A). The efficiency factor is then defined by η f = lσ ( f, ) zz l/2 l/2 Accepted Author Manuscript (DOI:0.06/j.compositesa ) σ ( zz (z) dz (2) Preprint submitted to Elsevier September 7, 20
2 where σ ( zz (z) is the average stress in the fibers and σ ( zz f, ) is the farfield fiber stress in the corresponding infinite concentric cylinders. The CCM problem is easily solved by shear lag analysis to give [, 2, 3]: tanh βρ η f = (3) βρ where β is the dimensionless shearlag parameter and ρ = l/d is the fiber aspect ratio (for fiber diameter d). Since tanh x for large x, this equation has the limiting solution: ρ(η β( η This limiting solution is accurate within % for η f 0.7. Thus, given any desired fiber efficiency and shear lag parameter, the fiber aspect ratio required to achieve that efficiency can easily be calculated. Here, % efficiency was arbitrarily selected as a benchmark for excellent shortfiber composites. The aspect ratio required to achieve this efficiency, denoted as ρ, is (4) ρ = 0 β (5) This same criterion was used by Hull and Clyne []. It would be possible to account for additional stress transfer into the fibers ends, but for stiff fibers (relative to the matrix), the effect is always small. The standard approach in the composites literature [, 2] has made aspect ratio calculations by using the shearlag parameter first derived by Cox [4]: β cox = 2 Gm which implies ρ (cox) E zz ( ln = 5 V f 2( + ν m ) ( ) E zz ( ln V f (6) E m where G m = E m /(2( + ν m )) is the shear modulus of the matrix and ν m is its Poisson s ratio. This approach has two serious deficiencies. First, ρ (cox) is independent of scale, which is a consequence of conventional elasticity analysis. A Coxbased analysis of nanofiber reinforced polymers is pointless because it would provide nothing new compared to analysis of conventional fibers. Second, the Cox shear lag parameter can be shown by comparison to FEA calculations to be very inaccurate [3, 5]. Aspect ratio requirements predicted by β cox are wrong by more than an order of magnitude. Shear lag analysis of fiber/matrix stress transfer can be much more accurate, such as the method first derived by Nayfeh [6] and later developed into modern stresstransfer theory by McCartney [7]. This improved shear lag solves the accuracy problem, but still has several deficiencies. First, the improved β is still scale invariant and thus provides no information unique to nanocomposites. Second, the analysis assumes a solid fiber and thus provides no information about hollow nanotubes. Third, the analysis breaks down at low fiber volume fracture and thus provides no guidance for work aimed at developing highperformance, lowfibervolumefraction nanocomposites. This paper uses recent advances in fiber/matrix shear lag analysis [3, 5, 8] that extend the NayfehMcCartney approach to solve its deficiencies. The new shearlag methods extend the analysis to handle multiple concentric cylinders and to handle a hollow core. This paper used these extensions to look at reinforcement effects of singlewall nanotubes (SWNT) and multiwall nanotubes (MWNT) as compared to solid carbon fibers. More importantly, the new shearlag methods can model imperfect interfaces (or interphases) between the matrix and the fiber or 2
3 between walls of a MWNT. The presence of an imperfect interphase introduces a scaling term that makes nanocomposites much different than conventional composites, and, for the first time, makes shear lag analysis a useful tool for modeling of nanofiber composites. The interface term reveals effects that may be detrimental to nanofiber reinforced composites. In other words, smalldiameter fibers put more burden on the interface than largediameter fibers. For effective nanofiber reinforcement, the interface must be excellent. Finally, the new shear lag methods have solved the issue of low fiber volume fractions. This feature was used to evaluate the potential for low V f nanocomposites with excellent properties. Such composites seem unlikely. Nanocomposite development would benefit more by emphasis on higher V f composites. 2. Shear Lag Theory First a remark. The fiberefficiencyadjusted rule of mixtures in Eq. () is a common first step in shortfiber composite analysis [, 2]. When η f is found by a CCM analysis, the result is an upper bound to E c. The CCM in Fig. A is a unit cell for a composite. When the CCM has the same V f as the bulk composite, the full composite consists of repeating unit cells as illustrated in Fig. B. But, the composite can be built from CCM unit cells in many ways. An alternative is to imagine the CCM unit cell as having fiber volume fraction V f that is higher than V f in the bulk composite. The full composite then consists of CCM unit cells interspersed with pure matrix cells of length l m = (V f V l/v f such that the total composite fiber volume fraction remains V f. The extreme geometry is when the CCM is pure fiber or V f = (see Fig. D). This last example has fiber and matrix elements in series that has the Reuss lower bound or series modulus. As V f decreases from to V f the modulus transitions from this lower bound to the upper bound result. All calculations in this paper used the upper bound result, i.e., used V f = V f. As a consequence, the η f calculated here is the upper bound to fiber efficiency, which implies that ρ is a lower bound to the required aspect ratio. The benchmark term ρ thus defines the minimum fiber aspect ratio needed for a particular short fiber composite to be highly efficient. But, since axial properties are usually well modeled by upper bound results [9], this approach should provide a useful benchmark. The CCM geometry for a SWNT in a matrix is shown in Fig. A. Here r 0 and r f are the inner and outer radii of the SWNT wall and r m is the outer radius of the matrix. The shear lag parameter, in dimensionless form and including imperfect interface effects is [3, 8]: β 2 = B r 2 f A (7) where A = B = 2G ( zr r2 0 O f (r) r 2 + ( r 2 ) m 2G m r I 2 m (r) + r f D ( f m) s 2 zz (r 2 f r2 0 ) + 2 E m (rm 2 r 2 (9) E ( (8) where G ( zr and G m are the fiber axial shear modulus (fiber is assumed orthotropic) and the matrix shear modulus (matrix is assumed isotropic), O f (r) and I m (r) are fiber and matrix shape functions, and D ( s f m) is an imperfect interface parameter for the fibermatrix interface. 3
4 σ 0 /V m z σ 0 /V m +l/2 0 r l/2 σ 0 /V m σ 0 /V m V f * = V f V f * > V f V f * = r 0 r f r m 0 A B C D Figure : A. Cylindrical coordinate system for concentric cylinders model analysis for a singlewall nanotube of radius r f (and core radius r 0 ) in a matrix cylinder of radius r m under total applied stress σ 0, which is applied only to the matrix. The single wall is shaded gray; the core and matrix are both white. B. A composite structure made of a repeating unit cells of matrix and fiber. C. A composite structure made up of repeating unit cells having V f > V f and regions of pure matrix such that the entire composite has fiber volume fraction V f. D. Same as C except V f =. The imperfect interface model is based on Hashin s approach to modeling interfaces in composites [0, ]. In brief, the modeled 2D fibermatrix interface is allowed to have a displacement discontinuity. In shear lag analysis the only discontinuity that applies is relative sliding between the fiber and matrix. This axial displacement discontinuity, [w], is then assumed to be proportional to the interfacial shear stress: [w] = τ rz(r f, z) D ( f m) s If D ( s f m), the discontinuity is zero and the interface is perfect. If D ( s f m) 0 the interfacial shear stress is zero and the interface is debonded. Values between 0 and define an imperfect characterizing the interface quality. This interface modeling converts a 3D interphase zone into a 2D interface, which simplifies analysis and reduces the number of unknown interphase properties. In other words, a model with a 2D interface having interface property D s gives approximate results for bulk composite response when compared to a model with an explicit 3D interphase. It achieves bulk response results with fewer interphase properties. If the real interphase zone has reduced stiffness (relative to fiber and matrix), the best 2D model would require a low D s corresponding to slippage in the 2D view. If the real interphase was interface with D ( f m) s divided into pure fiber and matrix, the 2D model would be correct with D s =. It is also conceivable that interactions between a fiber and a matrix might stiffen the interphase region. The best approximation to a stiffened interphase zone in a model that has only a 2D interface might need a negative D s. It is better viewed a /D ( s f m) that becomes zero for a perfect 2D interface, but may become negative for an interphase zone that is stiffened relative to other phases 4 (0)
5 [2] (note that negative D s values are energetically admissible provided they correspond to an interphase zone with finite stiffness [2], i.e., provided /D ( s f m) is greater than the result for a rigid interphase, which is negative). Note that the role of interfacial properties on nanocomposite properties has often been the subject of papers on nanocomposites modeling (e.g., [3, 4]), which usually have involved modifications of the Eshelby method for ellipsoidal inclusions [5] now with an interphase. The approach of this paper is to modify shear lag methods and account for interface effects using a single interfacial property, D s. This new approach allows many shearlag methods to be applied to nanocomposite modeling and reduces the role of the interface to a single property. As discussed below, it might be possible to measure D s by experiments. In contrast, some modeling methods have been based on interfacial properties that are unknown and difficult to measure. Furthermore, a analysis involving cylindrical fibers may be the preferred approach to modeling fiber aspect ratio effects rather then analyses based on elliptical inclusions. The functions O f (r) and I m (r) are shape functions for the fiber and matrix and the brackets (< >) indicate an average over the fiber or matrix crosssectional area. Any shape functions can be used with the only requirements being that O f (r 0 ) = 0, O f (r = I m (r =, and I m (r m ) = 0 [5]. McCartney suggested specific functions based on an assumed (and reasonable) radial dependence for the shear stress [7]: O f (r) = r2 r 2 0 r 2 f r2 0 and I m (r) = r2 m r 2 r 2 m r 2 f () After averaging, the shape function terms become: r2 0 O f (r) r 2 ( r 2 ) m r I 2 m (r) r0 2 r0 2 = r 2 f r2 0 r 2 f ln r2 f + r2 f r2 0 r2 0 r0 2 2r0 2 (2) = ( ) 2 ( ) φ φ 2 ln ( φ) (3) φ φ rm 2 rm 2 = rm 2 r 2 ln r2 m r2 m r 2 f f rm 2 r 2 f r 2 2r f m 2 (4) = ( Vm V m ) ln ( V m + χ) (5) V m where φ = (r 2 f r2 0 )/r2 f and V m = (r 2 m r 2 /r2 m. The χ term in the ln( V m +χ) term was included to make that term stable for V m close to. Finite element analysis (FEA) calculations show that χ = is a universal constant that works for stress transfer into both isotropic and anisotropic fibers and for any fiber/matrix modulus ratio [5]. The full shear lag parameter becomes β 2 = 4 G ( zr ( 2 ( φ φ V m E m V m + E ( zz φ ) 2 ( ln ( φ) φ )) ( φ Vm G m V m V m ln ( V m + χ) ) + 2 r f D ( s f m) (6) 5
6 Thus, the aspect ratio to get % efficiency from the fibers is ρ = 5 f (φ) E( zz G ( zr + 2( + ν m ) f 2 (V E( zz V f E ( zz V f E m + φ f (φ) = ( ) 2 ( ) φ φ 2 ln ( φ) φ φ ( f 2 (V = V f E m + 2E( zz r f D ( s f m) ( V ln ( V 2 f + χ ) ) (7) (8) (9) where ν m is the Poisson s ratio of the matrix. ρ was written to use V f and to emphasize key ratios, which are E zz ( /G ( zr, E zz ( /E m, and E zz ( /(r f D ( s f m) ). The last ratio is the only one that contains a scaling factor or a fiber radius effect. The function f (φ) decreases smoothly from 0.5 to 0.0 as φ decreases from (solid cylinders) to 0 (thinwalled cylinder). The function f 2 (V decreases smoothly from 3.2 to 0.0 as V f increases from 0 to. This function needs χ = for evaluation at V f = 0, but χ should be changed to zero for V f > 0.5. All calculations in this paper were for V f < 0.5 and thus χ was kept at This author is biased that the shearlag parameter from his work [3, 8], which is a extension of prior cylindrical shear lag models by Nayfeh [6] and McCartney [7] to include hollow fibers, to work at low V f, and to model an imperfect interface, is the preferred shear lag model. This bias can be justified by the interface term, which introduces scaling effects and makes a shearlag analysis worthwhile, and by its accuracy, which can be evaluated by comparison to finite element calculations (FEA). The average fiber stress from a shear lag analysis is [8] σ ( zz (z) σ ( f, ) zz = cosh βz r f cosh βρ This analytical solution is compared to FEA results for a hollow fiber in Fig. 2. The FEA comparison confirms that the shear lag analysis using β in Eq. (6) is extremely accurate for axial stresses and for both perfect and imperfect interfaces. The FEA analysis with an imperfect interface used the same Hashin [0, ] interface model by using elements described in Ref. [2]. The normalizing farfield fiber stress was found by concentric cylinders analysis of infinite cylinders [9] (see the appendix). Since the shear lag β in Eq. (6) is accurate, alternative shear lag parameters that differ are, by definition, inaccurate and should be avoided. One notable alternative parameter is found in the original (and oftencited) fiber/matrix shear lag analysis by Cox [4] (see Eq. (6)). Because β cox is significantly smaller then β in Eq. (6), it predicts aspect ratio requirements that are an order of magnitude or more too high (depending on V. In brief, no new shearlag application should be trusted until it is verified by FEA. The shear lag parameter used here was verified; the Cox parameter is inaccurate and therefore should never be used. Some limiting results were found useful. First, most reinforcement is done by fibers that are much stiffer than the matrix. The stifffiber limit, defined as E zz ( φ >> E m and G ( zr >> E m, is ρ (stiff) = lim E m <<E zz ( φ, G ( zr 2E m ρ = f r f D ( s f m) 2 (V ( + ν m ) 6 (20) V f V f (2)
7 20 Fiber Stress (%) (fm) D s = (fm) r f D s = 300 (fm) r f D s = 00 Φ = 0.75 Shear Lag FEA Position (fiber diams) Figure 2: Average axial fiber stress (as percent of farfield fiber stress) as a function of position (in units of fiber diameters) by shearlag analysis (solid curves) or by finite element analysis (dashed curves). The three curves are for three different values of r f D ( s f m) in units of MPa. These calculations used E m = 2500 MPa, ν m = 0.33, E zz ( /E m = 400, E zz ( /G ( zr = 0, r f = µm, r 0 = 0.5 µm, φ = 0.75, ρ = 50, and V f = This stiff limit depends only on matrix properties, the interface quality, and the fiber radius. It is independent of other fiber properties including whether the fiber is solid or hollow (i.e., independent of φ). This stifffiber limit is infinite as V f 0, but the full Eq. (7) is wellbehaved as V f 0 for any fiber stiffness. The result is: ρ (0) = lim ρ = 5 φ V f f (φ) E( zz ( + ν 0 G ( zr m ) E( zz + 2E( zz E m r f D ( s f m) (22) 3. Results 3.. Single Wall Nanotubes with Perfect Interface This section considers SWNTs compared to solid AS4 carbon fibers when the interface is perfect (D ( s f m) = ). When the interface is perfect, the shearlag parameter is scale invariant meaning the only differences between SWNTs and large, solid fibers are their moduli and the φ factor. The key SWNT properties are its radius and wall thickness and its tensile and shear moduli. Wall thickness estimates vary from nm to 0.69 nm [6]; here the thickness was assumed to be the interlayer graphite spacing or 0.34 nm [6]. The SWNT radius was set to r f = 0.75 nm or an average of SWNTs with diameters between and 2 nm. These assumptions resulted in r 0 = 0.4 and φ = Reports on the axial modulus of SWNTs vary from 220 GPa to 450 GPa [7]. All calculations here were for reinforcing a typical glassy polymer with E m = 2.5 GPa and ν m = 0.33; thus E zz ( /E m is between 88 and 660. The E zz ( /G zr ( ratio requires knowledge of the SWNT axial shear modulus, which is unknown (note: for orthotropic materials G ( zr is different than a shear modulus that could be determined by torsion experiments (i.e., G ( zθ ), but it might be similar). Here, E( zz /G ( zr was assumed to be the same as it is for solid AS4 carbon fibers or E zz ( /G ( zr = 220/4 = 5.7. This assumption had virtually no influence on the calculations and thus the E zz ( /G ( zr value is relatively unimportant. This observation might 7
8 Solid V f 0% 200 AS4 SWNT ρ 50 Hollow (ϕ=0.70) % 00 2% 50 5% 0% E (f) zz /E m Figure 3: The minimum fiber aspect ratio, ρ, as a function of E zz ( /E m for various fiber volume fractions. The two solid curves at each volume fraction are for solid fibers (φ = ) or hollow fibers (φ = 0.70) (using Eq. (7)). The dashed lines for V f % are the stiff fiber limit, ρ (stiff) (using Eq. (2)). The vertical dotted lines are expected E zz ( /E m ratios for AS4 or SWNT fibers. change if SWNTs were found to have an anomalously low G ( zr. The solid AS4 carbon fiber properties are r f = 3500 nm, E zz ( = 220 GPa, E zz ( /G ( zr = 5.7, and φ =. Figure 3 plots the minimum fiber aspect ratio (ρ ) as a function of E zz ( /E m for solid and hollow (with the assumed φ = 0.70) fibers for several volume fractions. The minimum aspect ratio increases as E zz ( /E m increases, but at a decreasing rate as V f increases. Comparing volume fractions, the fiber aspect ratio requirements are high for low V f, but decrease dramatically for higher V f. The horizontal dashed lines are the stiff fiber limits. Each volume fraction asymptotically approaches the stiff limit. For V f 5%, the stiff fiber limit gives a reasonable approximation for reinforcement by any stiff fiber. No stiff limit is plotted for V f 0% because lim V f 0 ρ (stiff) =. The figure instead plots ρ (0) ; this low V f limit shows the highest required fiber aspect ratio, which continues to increase as E zz ( /E m increases. Each volume fraction in Fig. 3 has one curve for solid fiber and another for hollow fiber. The solid curve is always slightly higher. The vertical dashed lines show possible E zz ( /E m for AS4 or SWNT fibers (with E zz ( = 250 GPa), respectively. Although the solid ρ curves are always higher than the hollow curves, the intersection of the AS4 properties with the solid curve is always lower than the intersection of the SWNT properties with the hollow curve. This difference, however, depends on V f the fiber aspect ratio intersections for SWNTs are essentially identical to those for AS4 fiber intersections for V f 5%, but are slightly higher for V f < 5%. The largest difference, which may reach a factor of 2, occurs in the limit as V f 0%. In other words, ρ is rather weakly dependent on φ except at low V f. ρ for SWNTs would decrease further if φ was less than 0.70 as assumed here, but within the range of possible SWNT shapes, the effect is expected to be small. The much larger effect of φ is as a scaling term in Eq. (), where contribution of SWNT modulus to composite modulus is directly reduced by any reduction in φ. The volume fraction effects for AS4 and SWNT fibers are plotted in Fig. 4. The three curves for D ( s f m) = are the perfect interface results. The AS4 and SWNT fiber aspect ratio requirements are virtually identical for V f 5%. For V f < 5%, SWNT composites would require slightly higher aspect ratio for excellent reinforcement. At high volume fractions (V f > 20%) 8
9 SWNT ρ AS4 D s (fm) = AS4 SWNT D s (fm) = Fiber Volume Fraction Figure 4: The minimum fiber aspect ratio, ρ, as a function of V f for AS4 and SWNT fibers. The D ( s f m) = curves are for a perfect interface. The D ( s f m) = (units of MPa/mm) curves are for an imperfect interface. The dashed lines are the stiff fiber limit, ρ (stiff). the fiber aspect ratios become rather modest ρ < 0; thus short fibers should reinforce more effectively at higher V f. The dashed line is the stiff fiber limit. It is an excellent approximation for SWNT for V f 2% and for AS4 for V f 5% Single Wall Nanotubes with Imperfect Interface The evaluation of imperfect interface effects requires knowledge of the interface parameter D ( s f m). The most direct way to measure D ( s f m) is to measure stress transfer into a single fiber. The results will resemble the axial stresses in Fig. 2. If the fiber and matrix properties are known, stress analysis can be used to determine D ( s f m). This technique was used on HM carbon fibers embedded in an epoxy matrix. The fiber axial strains were measured by Raman spectroscopy [8] and interpreted using a BesselFourier analysis [9] resulting in a measured r f D ( s f m) = 300 MPa [8] (note that D s in Refs. [8] and [9] is equivalent to r f D ( s f m) used here and defined by Hashin [0]). These same experimental results were reanalyzed by the shearlag analysis used here, which gave the same r f D ( s f m) = 300 MPa [5]. Using r f = 3.5 µm results in D ( s f m) = MPa/mm. Imperfect interface theory implies that D ( s f m) is an interface property that is independent of the fiber radius. There are no experimental results as a function of fiber radius, however, to know for sure. The following calculations assumed D ( s f m) is a material property and that it is the same for AS4 fibers and SWNTs as it is for HM fibers. Figure 4 plots the AS4 and SWNT fiber aspect ratio requirements with D ( s f m) = MPa/mm. An imperfect interface means that higher aspect ratios are needed before effective reinforcement can be realized. For AS4 fibers, ρ increased 2 4 fold, depending on V f. In contrast, for SWNTs, ρ increased fold, depending on V f. The dramatic effect for SWNTs is caused by their small r f, and the presence of r f in the denominator of the imperfect interface term. In brief, the interface effects with smalldiameter fibers, such as SWNTs, are much more prominent than in largerdiameter fibers. If the SWNT interface is similar to the HM fiber interface, then SWNTs are unlikely to ever produce effectively reinforced short fiber composites. 9
10 It is possible, however, that D ( s f m) for SWNTs may be dramatically different. First, D ( s f m) may not be a material property. The experiments needed to answer this question are to measure as a function of fiber radius for a series of otherwise identical fibers. Second, SWNTs may have much more favorable interactions with some matrices than HM fibers have with epoxy. For example a SWNT might constrain an interphase region inducing a stiffening effect that could result in a negative D ( s f m). If such an effect occurs, ρ would be similar to the perfect interface results, or perhaps slightly lower. Conversely, a negative interaction between a SWNT and a matrix that results in a compliant interphase would be an extremely poor choice for a nanofiber composite. Note that negative D ( s f m) values are limited to the condition that β remain real. Thus the physically accessible range for D ( s f m) is > r f f (φ) + f 2(V (23) D ( s f m) 2 G ( zr G m D ( f m) s The lower limit corresponds to instant stress transfer (i.e., a rigid interphase) with β = and ρ = Multiwall Nanotubes A MWNT shear lag analysis could be constructed using a model of multiple concentric cylinders and it could account for slippage (or telescoping) between the cylinders by adding an interface parameter for walltowall contact D (w w) s [3, 5]. Assuming the various walls have the same mechanical properties as a SWNT wall, the only new parameter would be D (w w) s. This complicated, multicylinder analysis, however, is unnecessary. The MWNT results would clearly fall between the SWNT results for outer wall only (if D (w w) s 0) and SWNT results that considered all walls as one solid wall (if D (w w) s ). Since the results in Figs. 3 and 4 show little effect on the diameter of the core, the MWNT fiber aspect ratio requirements must be virtually identical to those of SWNTs. Once the fiber aspect ratio requirements are met, the overall composite modulus depends on the product E zz ( φ. For SWNT, φ is calculated from radius and wall thickness. For MWNTs, the effective φ depends on D (w w) s. If the walls are free to slip, or telescope under strain, that would imply that D (w w) s 0. In this limit, the inner walls would carry no stress and the effective φ should be determined from r f and the inner radius of the outermost wall. On the other hand, if the walls are perfectly bonded, the effective φ should be calculated from r f and the inner radius of the innermost wall. For partial bonding the effective φ would be between these two limits. Most descriptions of MWNT suggest that slippage is more likely than perfect bonding. Thus composites of MWNTs are more likely to reinforce as if they were SWNTs made by removing the inner walls. 4. Discussion and Conclusions A simple shear lag analysis of concentric cylinders, when done accurately, provides useful results about fiber aspect ratio requirements in short fiber composites and about the effective modulus of aligned short fiber composites. A particularly simple result for aspect ratio is the stiff limit or ρ (stiff) (see Eq. (2)). This stiff limit is very accurate for V f > 5%. Even for V f < 5% it is sufficiently accurate that it gives useful results; it is probably not worth the effort to determine the extra material properties required to use the full ρ (see Eq. (7)). It cannot be used in the limit V f 0, but then ρ (0) (see Eq. (22)) can be used instead. Based on ρ(stiff), the fiber aspect ratio 0
11 requirement depends on fiber volume fraction. It is highest for low V f and decreases significantly at higher V f. The only fiber and matrix properties that affect ρ (stiff) are the group E m /(r f D ( s f m) ). This term is an interphase effect. The presence of r f in the denominator is a scaling effect that could be detrimental to nanocomposites. In other words, the interface quality is more important in nanocomposites than in composites with micron or larger sized fibers. One should not expect excellent SWNT composites unless /D ( s f m) is close to zero or slightly negative. Once aspect ratio requirements are met, the criterion used here implies that η f 0.9. The final composite modulus then depends on E m, V f and the product E zz ( φ (see Ec in Eq. ()), which is a reduced modulus that is more important to composite properties than is the wall modulus, E zz (. The reduced modulus can be determined from forcedisplacement experiments on SWNTs by normalizing to the entire crosssectional area rather then the area of the wall material (i.e., an easier experiment then determining E zz ( because it does not require determination of the wall thickness). For practical applications, E zz ( φ should be reported along with E zz ( results. For MWNTs, E zz ( φ should use an effective φ that accounts for contribution of the interior walls. This effective φ will be between the result based on the outer wall alone and the result that includes all walls. The Ec in Eq. () is for aligned, shortfiber composites, which are uncommon materials. But, given results for aligned shortfiber composites, 2D or 3D random composite properties can be evaluated by suitable 2D [20] and 3D [2] averaging methods. The resulting random composite moduli scale with Ec and thus calculations here are relevant to both aligned and random composites. Because Ec is an upper bound modulus, the averaging method also gives an upper bound for the random composite. By definition, an upper bound modulus is the highest possible modulus for all possible structures. In other words, all structures, including percolated geometries, must have a lower modulus. The idea that percolation can provide unexpected properties that violates upper bounds is a misconception. One claimed SWNT potential is that because of their remarkable moduli, they could produce stiff composites at very low fiber volume fraction. Fiber aspect ratio requirements, however, suggest this potential is unlikely to be realized. As V f decreases, the required aspect ratio increases. In the limit V f 0, it increases further as E zz ( increases. In other words, reinforcement is always less effective at low V f. Better potential for nanocomposites is more likely at higher V f, where the aspect requirements are much smaller ρ can be below 0 for V f around 25%. The interface is still critical, but favorable SWNT/matrix interactions might stiffen the interphase and lead to better composites than could be obtained with largerdiameter fibers. These low aspect ratio requirements at higher V f are lower than prior calculations for short fiber composites (e.g., ρ 00 [], which is too high because it used β cox ). Recall, however, that this new ρ is a lower bound. Real materials might require a higher aspect ratio, but the aspect ratio needed should decrease as V f increases. The importance of the interface and the lack of experimental results for D ( s f m) suggests it would be beneficial to develop a method to measure interface quality. The best experiment is to directly measure stress transfer into a single fiber using Raman methods [8]. That approach, however, only works for certain fibers and is beyond the resolution of Raman for SWNTs. One possible alternative would be to make a series of aligned shortfiber composites with varying fiber aspect ratio. Two options for characterizing the composites would be to measure the modulus or to use Raman to measure an average fiber strain. Either of these results would provide an experimental estimate of η f. With known fiber and matrix properties, the only unknown in η f would be the interfacial parameter.
12 Finally, this paper s analysis assumes that continuum mechanics for stress transfer applies to SWNTs. In other words, assuming continuum mechanics is appropriate, what can be said about the fiber aspect ratio requirements and composite modulus of SWNT reinforced polymers? Such modeling can guide nanocomposite development. Two key findings here are that fiber aspect ratio requirements are modest, but only at higher V f, and that the interface is important. Experiments should focus on higher V f composites and developing new interface characterization methods. The alternative is to assume that some undiscovered nano effect exists and therefore low V f composites with remarkable properties are possible. The nature of undiscovered phenomena, however, is that they might not exist or if they do exist, they might be detrimental rather then beneficial. Appendix The farfield fiber stress was found by a concentric cylinder analysis for infinite length cylinders [9] amended to allow for a hollow fiber. The FEA calculations here were done for a transversely isotropic fiber. The results for such fibers are σ ( f, ) zz = E A + 4ν AV m (ν A ν m ) V m kt + V f φ k m + φ G m φ G T σ app E A where EA is the effective axial modulus of the concentric cylinders: E A = E AV f φ + E m V m + 4V mv f φ(ν A ν m ) 2 V m kt + V f φ k m (24) (25) + φ G m φ G T Here σ app is the total applied stress, E A, ν A, k T, and G T are axial modulus, axial Poisson s ratio, transverse bulk modulus, and shear modulus of the transversely isotropic fiber and E m, ν m, k m, and G m are the same properties for the isotropic matrix. V f, V m, and φ are as defined in the text of this paper. In these equations, the first terms dominate while the second terms account for small effects due to Poisson s ratio difference between the fiber and the matrix. A similar analysis could be done for orthotropic fibers, but results in considerably more complicated expressions. The solid fiber results in Ref. [9] are recovered by setting φ = and eliminating the G T term. References [] D. Hull, T. W. Clyne, An Introduction to Composite Materials, 2nd Edition, Cambridge University Press, 996. [2] M. R. Piggott, Load Bearing Fibre Composites, 2nd Edition, Kluwer Academic Publishers, [3] J. A. Nairn, On the use of shearlag methods for analysis of stress transfer in unidirectional composites, Mech. of Materials 26 (997) [4] H. L. Cox, The elasticity and strength of paper and other fibrous materials, Brit. J. Appl. Phys. 3 (952) [5] J. A. Nairn, Generalized shearlag analysis including imperfect interfaces, Advanced Composite Letters 3 (2004) [6] A. H. Nayfeh, Thermomechanically induced interfacial stresses in fibrous composites, Fibre Sci. & Tech. 0 (977) [7] L. N. McCartney, Analytical models of stress transfer in unidirectional composites and crossply laminates, and their application to the prediction of matrix/transverse cracking, in: J. N. Reddy, K. L. Reifsnider (Eds.), Local Mechanics Concepts for Composite Material Systems, 992, pp [8] J. A. Nairn, D.A. Mendels, On the use of planar shearlag methods for stresstransfer analysis of multilayered composites, Mechanics of Materials 33 (200)
13 [9] Z. Hashin, Analysis of properties of fiber composites with anisotropic constituents, J. Appl. Mech. 46 (979) [0] Z. Hashin, Thermoelastic properties of fiber composites with imperfect interface, Mech. of Materials 8 (9) [] Z. Hashin, Extremum principles for elastic heterogenous media with imperfect interfaces and their application to bounding of effective moduli, Journal of the Mechanics and Physics of Solids 40 (4) (992) [2] J. A. Nairn, Numerical implementation of imperfect interfaces, Computational Materials Science 40 (2007) [3] H. L. Duan, J. Wang, Z. P. Huang, B. L. Karihaloo, Eshelby formalism for nanoinhomogeneities, Proc. Roy. Soc. Lond. A 46 ( ). [4] P. Sharma, S. Ganti, Sizedependent eshelby s tensor for embedded nanoinclusions incorporating surface/interface energies, Journal of Applied Mechanics 7 (5) (2004) doi:0.5/ URL [5] J. D. Eshelby, The determination of the elastic field of an ellipsoidal inclusion and related problems, Proc. R. Soc. Lond. A 24 (957) [6] Y. Huang, J. Wu, K. C. Hwang, Thickness of graphene and singlewall carbon nanotubes, Phys. Rev. B 74 (24) (2006) doi:0.03/physrevb [7] Y. Huang, R. J. Young, Interfacial micromechanics in thermoplastic and thermosetting matrix carbon fibre composites, Composites Part A 27A (996) [8] A. Paipetis, Y. C. Liu, C. Galiotis, J. A. Nairn, Stress transfer from the matrix to the fiber in a fragmentation test: Raman experiments and analytical modeling, J. Comp. Mat. 33 (999) [9] J. A. Nairn, Y. C. Liu, C. Galiotis, Analysis of stress transfer from the matrix to the fiber through an imperfect interface: Application to raman data and the singlefiber fragmentation test, in: C. J. Spragg, L. T. Drzal (Eds.), ASTM STP 2, 995, pp [20] J. Halpin, J. Kardos, Moduli of crystalline polymers employing composite theory, Journal of Applied Physics 43 (5) (972) doi:0.063/ [2] R. M. Christensen, Mechanics of Composite Materials, John Wiley & Sons, New York,
ANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULLOUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES
Advanced Composite Letters, Vol. 9, No. 6, 373383 000 Full Article ANALYTICAL FRACTURE MECHANICS ANALYSIS OF THE PULLOUT TEST INCLUDING THE EFFECTS OF FRICTION AND THERMAL STRESSES John A. Nairn Material
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationCHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement
CHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationNumerical Modeling and Experiments on the Role of StrandtoStrand Interface Quality on the Properties of Oriented Strand Board
Numerical Modeling and Experiments on the Role of StrandtoStrand Interface Quality on the Properties of Oriented Strand Board John A. Nairn (Professor) and Edward Le (PhD Student) Wood Science & Engineering,
More informationBen W. Kim 1 and John A. Nairn 2
J. Materials Science, submitted (2002) Author prepared reprint Experimental Verification of the Effects of Friction and Residual Stress on the Analysis of Interfacial Debonding and Toughness in Single
More informationThe stress transfer efficiency of a singlewalled carbon nanotube in epoxy matrix
JOURNAL OF MATERIALS SCIENCE 39 (2 004)4481 4486 The stress transfer efficiency of a singlewalled carbon nanotube in epoxy matrix K. Q. XIAO, L. C. ZHANG School of Aerospace, Mechanical and Mechatronic
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationFRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
Proc. 2 nd ESIS TC4 Conference on Polymers and Composites, in press, 1999 Author prepared reprint FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, TRACTIONLOADED CRACKS, AND IMPERFECT INTERFACES
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationCHAPTER 4 MODELING OF MECHANICAL PROPERTIES OF POLYMER COMPOSITES
CHAPTER 4 MODELING OF MECHANICAL PROPERTIES OF POLYMER COMPOSITES 4. Introduction Fillers added to polymer matrices as additives are generally intended for decreasing the cost (by increase in bulk) of
More informationFRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, IMPERFECT INTERFACES, AND TRACTIONLOADED CRACKS
Composites Science and Technology, 61, 159167 (000) c 000 Elsevier Science Limited Author Prepared Preprint. All rights reserved ELSEVIER FRACTURE MECHANICS OF COMPOSITES WITH RESIDUAL STRESSES, IMPERFECT
More informationDevelopment of a code to generate randomly distributed short fiber composites to estimate mechanical properties using FEM
International Journal of Theoretical and Applied Mechanics. ISSN 09736085 Volume 12, Number 4 (2017) pp. 863872 Research India Publications http://www.ripublication.com Development of a code to generate
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationAnalytical and experimental methods for a fracture mechanics interpretation of the microbond test including the effects friction and thermal stresses
International Journal of Adhesion & Adhesives 19 (1999) 59 7 Analytical and experimental methods for a fracture mechanics interpretation of the microbond test including the effects friction and thermal
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationMicromechanical analysis of FRP hybrid composite lamina for inplane transverse loading
Indian Journal of Engineering & Materials Sciences Vol. 15, October 2008, pp. 382390 Micromechanical analysis of FRP hybrid composite lamina for inplane transverse loading K Sivaji Babu a *, K Mohana
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationThe effect of interfacial bonding on the damping behavior of nanocomposites
The effect of interfacial bonding on the damping behavior of nanocomposites Literature review The rapid and continuous growth in aerospace, automotive, and military applications requires special materials
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationStiffness Predictions for Unidirectional ShortFiber Composites: Review and Evaluation
Stiffness Predictions for Unidirectional ShortFiber Composites: Review and Evaluation Charles L. Tucker III Department of Mechanical and Industrial Engineering University of Illinois at UrbanaChampaign
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationA simple planestrain solution for functionally graded multilayered isotropic cylinders
Structural Engineering and Mechanics, Vol. 24, o. 6 (2006) 000000 1 A simple planestrain solution for functionally graded multilayered isotropic cylinders E. Pan Department of Civil Engineering, The
More informationMicrocracking, MicrocrackInduced. Delamination, and Longitudinal
NASA Contractor Final Report Microcracking, MicrocrackInduced Delamination, and Longitudinal Splitting of Advanced Composite Structures John A. Nairn University of Utah Salt Lake City, Utah Prepared for
More informationModeling Imperfect Interfaces in the Material Point Method using Multimaterial Methods
Copyright 2013 Tech Science Press CMES, vol.92, no.3, pp.271299, 2013 Modeling Imperfect Interfaces in the Material Point Method using Multimaterial Methods J. A. Nairn 1 Abstract: The multimaterial version
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationInterface properties between a steel prestressing strand and an epoxy matrix.
Interface properties between a steel prestressing strand and an epoxy matrix. J. Van Vooren 1, B. Van Vooren 2, D. Van Hemelrijck 1, 1 Free University of Brussel, Dept. of Mechanics of Materials and Constructions,
More informationPredicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics
Predicting Elastic Properties of Unidirectional SU8/ZnO Nanocomposites using COMSOL Multiphysics Neelam Mishra 1, and Kaushik Das *1 1 School of Minerals Metallurgical and Materials Engineering, Indian
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationA SHEARLAG ANALYSIS OF STRESS TRANSFER THROUGH A COHESIVE FIBREMATRIX INTERFACE
2 st International Conference on Composite Materials Xi an, 2025 th August 207 A SHEARLAG ANALYSIS OF STRESS TRANSFER THROUGH A COHESIVE FIBREMATRIX INTERFACE Zuorong Chen and Wenyi Yan 2 CSIRO Energy
More informationComposite angle ply laminates and netting analysis
10.1098/rspa.2002.1066 FirstCite epublishing Composite angle ply laminates and netting analysis By J. T. Evans and A. G. Gibson School of Mechanical and Systems Engineering, University of Newcastle upon
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationContinuum Modeling Techniques to Determine Mechanical Properties of Nanocomposites
International OPEN ACCESS Journal Of Modern Engineering Research (IJMER) Continuum Modeling Techniques to Determine Mechanical Properties of Nanocomposites Sonali Gholap 1, Dr. Dhananjay R. Panchagade
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationThe Rotating Inhomogeneous Elastic Cylinders of. VariableThickness and Density
Applied Mathematics & Information Sciences 23 2008, 237 257 An International Journal c 2008 Dixie W Publishing Corporation, U. S. A. The Rotating Inhomogeneous Elastic Cylinders of VariableThickness and
More informationHysteretic equivalent continuum model of nanocomposites with interfacial stickslip
Hysteretic equivalent continuum model of nanocomposites with interfacial stickslip Giovanni Formica 1, Michela Talò, Walter Lacarbonara 1 Dipartimento di Architettura, Università degli Studi Roma Tre
More informationMechanical Properties of Fiber Reinforced Composites Using Buckminster Fullerene Reinforcement
IJRMET Vo l. 4, Is s u e Sp l  1, No v 2013 Ap r i l 2014 ISSN : 22495762 (Online ISSN : 22495770 (Print Mechanical Properties of Fiber Reinforced Composites Using Buckminster Fullerene Reinforcement
More informationSensitivity studies on the shear lag parameter β using analytical and numerical techniques
Rowan University Rowan Digital Works Theses and Dissertations 8222016 Sensitivity studies on the shear lag parameter β using analytical and numerical techniques George Thomas Avery Rowan University,
More informationGraduate School of Engineering, Kyoto University, Kyoto daigakukatsura, Nishikyoku, Kyoto, Japan.
On relationship between contact surface rigidity and harmonic generation behavior in composite materials with mechanical nonlinearity at fibermatrix interface (Singapore November 2017) N. Matsuda, K.
More informationU.S. South America Workshop. Mechanics and Advanced Materials Research and Education. Rio de Janeiro, Brazil. August 2 6, Steven L.
Computational Modeling of Composite and Functionally Graded Materials U.S. South America Workshop Mechanics and Advanced Materials Research and Education Rio de Janeiro, Brazil August 2 6, 2002 Steven
More informationDepartment of Mechanical Engineering, National Institute of Technology Rourkela, Rourkela , India
Composites, Article ID 629175, 12 pages http://dx.doi.org/10.1155/2014/629175 Research Article Effect of Fiber Geometry and Representative Volume Element on Elastic and Thermal Properties of Unidirectional
More informationLaminated Composite Plates and Shells
Jianqiao Ye Laminated Composite Plates and Shells 3D Modelling With 62 Figures Springer Table of Contents 1. Introduction to Composite Materials 1 1.1 Introduction 1 1.2 Classification of Composite Materials
More informationEFFECT OF INTERPHASE CHARACTERISTIC AND PROPERTY ON AXIAL MODULUS OF CARBON NANOTUBE BASED COMPOSITES
15 EFFECT OF INTERPHASE CHARACTERISTIC AND PROPERTY ON AXIAL MODULUS OF CARBON NANOTUBE BASED COMPOSITES Md. Abdulla Al Masud and A.K.M. Masud * Department of Industrial and Production Engineering, Bangladesh
More informationDistributed: Wednesday, March 17, 2004
MASSACHUSETTS INSTITUTE OF TECHNOLOGY DEPARTMENT OF MECHANICAL ENGINEERING CAMBRIDGE, MASSACHUSETTS 019.00 MECHANICS AND MATERIALS II QUIZ I SOLUTIONS Distributed: Wednesday, March 17, 004 This quiz consists
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationTHE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS THE MUTUAL EFFECTS OF SHEAR AND TRANSVERSE DAMAGE IN POLYMERIC COMPOSITES L.V. Smith 1 *, M. Salavatian 1 1 School of Mechanical and Materials
More informationExercise: concepts from chapter 8
Reading: Fundamentals of Structural Geology, Ch 8 1) The following exercises explore elementary concepts associated with a linear elastic material that is isotropic and homogeneous with respect to elastic
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationFracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load
Fracture Behaviour of FRP CrossPly Laminate With Embedded Delamination Subjected To Transverse Load Sriram Chintapalli 1, S.Srilakshmi 1 1 Dept. of Mech. Engg., P. V. P. Siddhartha Institute of Technology.
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationFinite Element Modeling of Residual Thermal Stresses in FiberReinforced Composites Using Different Representative Volume Elements
Proceedings o the World Congress on Engineering 21 Vol II WCE 21, June 3  July 2, 21, London, U.K. Finite Element Modeling o Residual Thermal Stresses in FiberReinorced Composites Using Dierent Representative
More informationUNLOADING OF AN ELASTICPLASTIC LOADED SPHERICAL CONTACT
2004 AIMETA International Tribology Conference, September 1417, 2004, Rome, Italy UNLOADING OF AN ELASTICPLASTIC LOADED SPHERICAL CONTACT Yuri KLIGERMAN( ), Yuri Kadin( ), Izhak ETSION( ) Faculty of
More informationPractice Final Examination. Please initial the statement below to show that you have read it
EN175: Advanced Mechanics of Solids Practice Final Examination School of Engineering Brown University NAME: General Instructions No collaboration of any kind is permitted on this examination. You may use
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationXI. NANOMECHANICS OF GRAPHENE
XI. NANOMECHANICS OF GRAPHENE Carbon is an element of extraordinary properties. The carboncarbon bond possesses large magnitude cohesive strength through its covalent bonds. Elemental carbon appears in
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationA micromechanical model for effective elastic properties of particulate composites with imperfect interfacial bonds
International Journal of Solids and Structures 42 (2005) 4179 4191 www.elsevier.com/locate/ijsolstr A micromechanical model for effective elastic properties of particulate composites with imperfect interfacial
More informationFracture Mechanics Analysis of Composite Microcracking: Experimental Results in Fatigue
Proceedings of the 5 th Technical Conference on Composite Materials, American Society of Composites, East Lansing, Michigan, June 1114, 1990). Fracture Mechanics Analysis of Composite Microcracking: Experimental
More informationSSNEMS Internal Report
E.3. Nanotube Reinforced Piezoelectric Polymeric Composites Subjected to ElectroThermo Mechanical Loadings Understanding the stress transfer between nanotube reinforcements and surrounding matrix is
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationAERO 214. Lab II. Measurement of elastic moduli using bending of beams and torsion of bars
AERO 214 Lab II. Measurement of elastic moduli using bending of beams and torsion of bars BENDING EXPERIMENT Introduction Flexural properties of materials are of interest to engineers in many different
More informationEffects of Fracture Parameters in an Anisotropy Model on PWave Azimuthal Amplitude Responses
PROC. ITB Eng. Science Vol. 38 B, No. 2, 2006, 159170 159 Effects of Fracture Parameters in an Anisotropy Model on PWave Azimuthal Amplitude Responses Fatkhan Program Studi Teknik Geofisika FIKTMITB
More informationMechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method
, pp.6782 http://dx.doi.org/1.14257/ijast.215.78.6 Mechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method P. Prasanthi
More informationApplicability of Engineering Models in Multiscale Modeling of Natural Fiber Hygro Elastic Properties
Applicability of Engineering Models in Multiscale Modeling of Natural Fiber Hygro Elastic Properties Janis Varna and Eri Marlund Department of Applied Physics and Mechanical Engineering Where is Luleå?
More informationNumerical Implementation of Imperfect Interfaces
Numerical Implementation of Imperfect Interfaces John A. Nairn Wood Science & Engineering, Oregon State University, Corvallis, OR, 97331, USA Abstract One approach to characterizing interfacial stiffness
More informationDebonding process in composites using BEM
Boundary Elements XXVII 331 Debonding process in composites using BEM P. Prochazka & M. Valek Czech Technical University, Prague, Czech Republic Abstract The paper deals with the debonding fibermatrix
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationDEVELOPMENT OF A MICROMECHANICAL MODEL IN INTERACTION WITH PARAMETERS RELATED TO THE MICROSTRUCTURE OF CARBON/EPOXY COMPOSITES
ECCM1616 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 2226 June 2014 DEVELOPMENT OF A MICROMECHANICAL MODEL IN INTERACTION WITH PARAMETERS RELATED TO THE MICROSTRUCTURE OF CARBON/EPOXY
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationInternational Journal of Engineering Science
International Journal of Engineering Science 63 (2013) 1 9 Contents lists available at SciVerse ScienceDirect International Journal of Engineering Science journal homepage: www.elsevier.com/locate/ijengsci
More informationAn ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials
An ElastoViscoPlastic Multiscale Model for Fibrous Unidirectional Composite Materials by Shari Lynn King A thesis presented to the University of Waterloo in fulfillment of the thesis requirement for
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationMECHANICS OF CARBON NANOTUBE BASED COMPOSITES WITH MOLECULAR DYNAMICS AND MORI TANAKA METHODS. Vinu Unnithan and J. N. Reddy
MECHANICS OF CARBON NANOTUBE BASED COMPOSITES WITH MOLECULAR DYNAMICS AND MORI TANAKA METHODS Vinu Unnithan and J. N. Reddy USSouth American Workshop: Mechanics and Advanced Materials Research and Education
More informationTensile Properties of ThermoplasticLaminated Composites Based on a Polypropylene Matrix Reinforced with Continuous Twaron Fibers
Tensile Properties of ThermoplasticLaminated Composites Based on a Polypropylene Matrix Reinforced with Continuous Twaron Fibers J. L. MENATUN, P. I. GONZALEZCHI Centro de Investigación Científica de
More informationMICROSTRUCTURAL AND ELASTIC PROPERTIES OF SHORT FIBER REINFORCED COMPOSITES
MICROTRUCTURAL AND ELATIC PROPERTIE OF HORT FIBER REINFORCED COMPOITE V. Müller 1, T. Böhlke 1 1 Institute of Engineering Mechanics, Chair for Continuum Mechanics, Karlsruhe Institute of Technology (KIT)
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationMODELLING THE THERMOELASTIC PROPERTIES OF SHORT FIBRE COMPOSITES WITH ANISOTROPIC PHASES
MODELLING THE THERMOELASTIC PROPERTIES OF SHORT FIBRE COMPOSITES WITH ANISOTROPIC PHASES P.J.Hine*, C.D.Price*, B.Whiteside $, A.M.Cunha # and I.M.Ward* *  IRC in Polymer Science and Technology, University
More informationEffect of Interlayers on Mechanical Properties and Interfacial Stress Transfer of 2D Layered Graphene Polymer Nanocompsites
University of Kentucky UKnowledge Theses and DissertationsMechanical Engineering Mechanical Engineering 2017 Effect of Interlayers on Mechanical Properties and Interfacial Stress Transfer of 2D Layered
More informationEffect of fibre shape on transverse thermal conductivity of unidirectional composites
Sādhanā Vol. 4, Part 2, April 25, pp. 53 53. c Indian Academy of Sciences Effect of fibre shape on transverse thermal conductivity of unidirectional composites B RAGHAVA RAO,, V RAMACHANDRA RAJU 2 and
More informationCalculation of Damagedependent Directional Failure Indices from the TsaiWu Static Failure Criterion
Van Paepegem, W. and Degrieck, J. (3. alculation of Damagedependent Directional Failure Indices from the saiwu Static Failure riterion. omposites Science and echnology, 63(, 353. alculation of Damagedependent
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationInteraction of Two Parallel Short Fibers in the Matrix at Loss of Stability
Copyright c 2006 Tech Science Press CMES, vol.13, no.3, pp.165169, 2006 Interaction of Two Parallel Short Fibers in the Matrix at Loss of Stability A.N.Guz and V.A.Dekret 1 Abstract: Stability problem
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationOpenhole compressive strength prediction of CFRP composite laminates
Openhole compressive strength prediction of CFRP composite laminates O. İnal 1, A. Ataş 2,* 1 Department of Mechanical Engineering, Balikesir University, Balikesir, 10145, Turkey, inal@balikesir.edu.tr
More informationANALYSIS OF THE SINGLEFIBRE FRAGMENTATION. D.A. Mendels
NPL REPORT MATC(A) I 7 ANALYSIS OF THE SINGLEFIBRE FRAGMENTATION TEST D.A. Mendels NPL Materials Centre National Physical Laboratory Teddington, Middlesex United Kingdom, TWll OL W Abstract This work
More informationInterfacial partial debonding and its in uence on the elasticity of a twophase composite
Mechanics of Materials 32 (2000) 695±709 www.elsevier.com/locate/mechmat Interfacial partial debonding and its in uence on the elasticity of a twophase composite S.F. Zheng, M. Denda, G.J. Weng * Department
More informationFinite Element and Plate Theory Modeling of Acoustic Emission Waveforms. NASA Langley Research Center. Hampton, VA *University of Denver
Finite Element and Plate Theory Modeling of Acoustic Emission Waveforms W. H. Prosser, M. A. Hamstad + *, J. Gary +, and A. O Gallagher + NASA Langley Research Center Hampton, VA 236811 *University of
More informationASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS
ASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS Dieter H. Pahr and Helmut J. Böhm Institute of Lightweight Design and Structural
More informationMechanics of wafer bonding: Effect of clamping
JOURNAL OF APPLIED PHYSICS VOLUME 95, NUMBER 1 1 JANUARY 2004 Mechanics of wafer bonding: Effect of clamping K. T. Turner a) Massachusetts Institute of Technology, Cambridge, Massachusetts 0219 M. D. Thouless
More informationSimulation of Cure Volume Shrinkage Stresses on Carbon/Vinyl Ester Composites in Microindentation Testing
8 th International LSDYNA Users Conference Simulation Technology (3) Simulation of Cure Volume Shrinkage Stresses on Carbon/Vinyl Ester Composites in Microindentation Testing Tom Mase, Lanhong Xu, Lawrence
More informationModule 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus
Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More information